Combined Use of Polyurethane Prepolymer and Aromatic Oil in Physicochemical Rejuvenation of Aged SBS Modified Bitumen for Performance Recovery

The high-quality reutilization of waste styrene–butadiene–styrene copolymer (SBS) modified asphalt mixtures is a difficult issue in the field of highways today, and the main reason is that conventional rejuvenation technology fails to achieve the effective rejuvenation of aged SBS in binder, causing significant deterioration in the high-temperature performance of the rejuvenated mixture. In view of this, this study proposed a physicochemical rejuvenation process using a reactive single-component polyurethane (PU) prepolymer as the repairing substance for structural reconstruction and aromatic oil (AO) as a common rejuvenator used to supplement the lost light fractions of asphalt molecules in aged SBSmB, according to the characteristics of oxidative degradation products of SBS. The joint rejuvenation of aged SBS modified bitumen (aSBSmB) by PU and AO was investigated based on Fourier transform infrared Spectroscopy, Brookfield rotational viscosity, linear amplitude sweep, and dynamic shear rheometer tests. The results show that 3 wt% PU can completely react with the oxidation degradation products of SBS and rebuild its structure, while AO mainly acted as an inert component to increase the content of aromatic components, thereby reasonably adjusting the compatibility of chemical components of aSBSmB. Compared with the PU reaction-rejuvenated binder, the 3 wt% PU/10 wt% AO rejuvenated binder had a lower high-temperature viscosity for better workability. The chemical reaction between PU and SBS degradation products dominated in the high-temperature stability of rejuvenated SBSmB and had a negative impact on its fatigue resistance, while the joint rejuvenation of 3 wt% PU and 10 wt% AO not only gave a better high-temperature property to aged SBSmB but could also have the capacity to improve its fatigue resistance. Compared to virgin SBSmB, PU/AO rejuvenated SBSmB has comparative low-temperature viscoelastic behavior characteristics and a much better resistance to medium-high-temperature elastic deformation.


Introduction
With the continuous development of highway construction, asphalt pavement has become the mainstream road surface in China due to its advantages of comfortable driving, low noise, and easy maintenance [1][2][3]. As ordinary petroleum asphalt pavement is prone to aging in the natural environment, it is prone to ruts, pits, and other damage under the repeated action of different traffic loads and is destroyed before reaching the design life [4][5][6]. In order to prolong the service life of ordinary asphalt pavement, the polymer styrene-butadiene-styrene (SBS) has been used on a large scale to prepare modified bitumen in expressways and other high-grade roads in China in the past 20 years, so as to improve the overall performance of asphalt pavement, especially resistance to deformation at high temperature and cracking at low temperature [7][8][9].
It is well recognized that the addition of modifiers such as SBS into virgin bitumen can improve its high-temperature rutting resistance, low-temperature cracking resistance, of permeable asphalt pavement. This indicates that PU modified asphalt mixture has good comprehensive performance after curing in air [38]. Therefore, PU prepolymer has excellent reaction potential to rebuild the molecular structure of aged SBS in order to improve the high-temperature properties of physically rejuvenated SBSmB.
In order to develop a rejuvenator that can not only rejuvenate the properties of aged bitumen but also the structure and properties of the SBS modifier, this study proposed a new physicochemical rejuvenation method based on the main reconstruction of the molecular structure of aged SBS. PU prepolymer was used as a reactive rejuvenator to react with active oxygen-containing groups, and AO was used as the bitumen component-returning agent to adjust the chemical composition of aged SBS modified bitumen. The effect of synergistic reaction rejuvenation of single-component polyurethane and aromatic oil on the structure and properties of aged SBS modified bitumen was evaluated by means of Fourier transform infrared (FTIR) spectroscopy, Brookfield rotational viscosity tests, linear amplitude sweep (LAS) tests [39] and dynamic shear rheometer (DSR) tests. The research flowchart of this study is presented in Figure 1.
Single-component polyurethane (PU) is a type of resin with an active isocyanate terminal group (-NCO) [33,34]. It can react with substances (including water) containing -OH without the assistance of curing agents to form polymers with excellent properties [35][36][37]. Lu et al. [38] used polyurethane modified bitumen to prepare permeable bitumen mixture, and found that it had better bonding strength, permeability, and mechanical properties than traditional permeable asphalt pavement, and solved the problem of long service life of permeable asphalt pavement. This indicates that PU modified asphalt mixture has good comprehensive performance after curing in air [38]. Therefore, PU prepolymer has excellent reaction potential to rebuild the molecular structure of aged SBS in order to improve the high-temperature properties of physically rejuvenated SBSmB.
In order to develop a rejuvenator that can not only rejuvenate the properties of aged bitumen but also the structure and properties of the SBS modifier, this study proposed a new physicochemical rejuvenation method based on the main reconstruction of the molecular structure of aged SBS. PU prepolymer was used as a reactive rejuvenator to react with active oxygen-containing groups, and AO was used as the bitumen component-returning agent to adjust the chemical composition of aged SBS modified bitumen. The effect of synergistic reaction rejuvenation of single-component polyurethane and aromatic oil on the structure and properties of aged SBS modified bitumen was evaluated by means of Fourier transform infrared (FTIR) spectroscopy, Brookfield rotational viscosity tests, linear amplitude sweep (LAS) tests [39] and dynamic shear rheometer (DSR) tests. The research flowchart of this study is presented in Figure 1.

SBS Modified Bitumen
The SBS modified bitumen (SBSmB) used in this study was a commercial product with a high temperature performance grade of PG76, and the modifier was added at approximately 4 wt%. The detailed physical properties are shown in Table 1. The SBS modified bitumen (SBSmB) used in this study was a commercial product with a high temperature performance grade of PG76, and the modifier was added at approximately 4 wt%. The detailed physical properties are shown in Table 1. In this study, single-component polyurethane (prepolymer) was used as the repairing substance for structural reconstruction of aged SBSmB, as it is able to reconstruct the molecular structure of SBS degradation products to some extent, thereby improving the overall performance of rejuvenated SBSmB. The PU prepolymer has a special molecular structure, with terminal isocyanate groups (-NCO), and is proven to have a strong reaction activity with -OH, -COOH, etc. The general formula of the chemical reaction between PU prepolymer and alcohol, carboxylic acid or water is presented below: AO (aromatics/the total, ≥80%) was economically obtained from industrial markets and used as a common bitumen rejuvenator for aSBSmB to adjust the aging-induced unbalanced chemical composition of bitumen for improved workability. The relevant technical indexes of AO are: brown appearance by visual inspection, density of 1.05 g/cm 3 , and flash point exceeding 200 • C.

Preparation of Aged SBSmB
The aging of SBSmB was carried out in an air-circulating oven at 163 • C for 48 h. After aging, aSBSmB was obtained and tested through a series of physical and rheological tests. Some of the performance results are shown in Table 1.

Preparation of Rejuvenated SBSmB
To prepare the PU rejuvenated SBSmB (3PU/aSBSmB), 3 wt% PU by weight was added to and mixed with aSBSmB at 170 • C for 5 min. In addition, 10 wt% AO was added to 3PU/aSBSmB under the same preparation conditions to prepare the jointly rejuvenated SBSmB, namely 3PU/10AO/aSBSmB. For the dosage adoption, this is because 3 wt% PU can chemically consume all the SBS degradation products in the aged SBSmB binder, and 10 wt% AO can achieve an optimum viscosity-reducing effect on the aged binder in the preliminary study.

Fourier Transform Infrared Spectroscopy (FTIR) Test
In this study, the NicoletTM iS50 FTIR instrument was used to test and analyze the molecular structure of the target bitumen samples, and to clarify whether PU prepolymer was able to react with aSBSmB. The attenuated total reflection method was used during the test, and the conditions were set as follows: the wave number range was 4000~400 cm −1 , scanning number was 32 times, and the resolution was 4 cm −1 . Different specimens of the same binder were tested twice for more accurate results, and the test was repeated more once if the two test results were not close.

Brookfield Rotational Viscosity Test
In accordance with ASTM D4402, the viscosity of bitumen samples was measured using the NDJ-1C Brinell rotational viscometer for virgin, aged and rejuvenated SBSmB at different temperatures, with the No. 27 rotor and a 50 rpm speed being selected for the test. Two or more viscosity tests were conducted on different specimens of the same binder, and the average value of the closest results which met the requirements of the allowable test error was taken as the measured value. The test temperatures were selected as 135 • C, 150 • C, 160 • C, 170 • C, and 180 • C. When processing the test data, Saal formula was used to linearly fit the viscosity-temperature curves. The Saal formula, recommended by the requirements of ASTM D2493, is an important linear expression to describe the viscosity-temperature characteristics of asphalt binder, as shown in Equation (1). According to the slope of the fitted curve, the temperature sensitivity of asphalt binder can be judged.
where, η is the value of viscosity, Pa·s; m is the regression coefficient, equal to the slope of the viscosity-temperature regression curve; n is the value of viscosity when the temperature of asphalt binder is zero; and T is Celsius, • C.

Linear Amplitude Sweep (LAS) Tests
LAS is a fatigue test method based on the viscoelastic continuum damage theory. To conduct this test, the DSR device was employed with 8 mm parallel plates and a controlled gap distance at 2 mm. The test was performed following two stages, namely, frequency sweep and amplitude sweep. For the first stage, the frequency sweep test for each sample was performed at 25 • C with an applied stress of 0.1% strain over a range of 0.1~30 Hz. For the second stage, the amplitude sweep test was run at the same temperature in a straincontrol mode at 10 Hz, and the loading scheme consisted of 10 s intervals of constant strain amplitude from 0.1% to 30%. The test for the same sample was repeated twice for error reduction. The performance parameter α of the material without damage is obtained from the frequency sweep test to calculate the parameter B in the fatigue equation. Combined with the amplitude sweep test results, the fatigue equation parameter A can be obtained, and the fatigue life N f can be also determined, accordingly.
The damage accumulation of the sample in the LAS test was calculated using Equation (2).
is the integrity parameter; G * is the complex shear modulus, MPa; γ i is the applied strain at t i time, %; t is the testing time, s; and α = 1 m is the rheological parameter of bitumen, where m is the slope of the best-fit straight line with log (storage modulus) on the vertical axis and log (applied frequency) on the horizontal axis.
For a specific time t, the relationship between C t and D t is as follows: The value of D t at fatigue failure is D f , calculated as follows: where, C peakstress is the value of the C(t) corresponding to the peak shear stress. The binder fatigue performance parameter N f can be calculated as follows: where, f is loading frequency, equal to 10 Hz; and k = 1 + (1 − C 2 )α; B = 2α; γ max is estimated maximum strain of pavement.

Dynamic Shear Rheometer (DSR) Tests
In this study, the rheological properties of bitumen samples were tested by MCR 702 DSR instrument, and the rheological parameters, such as complex modulus (G*), phase angle (δ), elastic modulus (G ) and viscous modulus (G"), were obtained. The test was repeated twice or more for different specimens of the sample binder to guarantee the accuracy of the results. The testing process was as follows: (1) rutting factor (G*/sin δ), for characterizing the high-temperature deformation resistance of bitumen samples, was tested using a pair of 25 mm parallel plates with a 1 mm gap at a control strain of 10%, an angular frequency of 10 rad/s, and a temperature of 76 • C; (2) fatigue failure temperature, for characterizing the fatigue resistance of bitumen samples, was determined by the temperature related to the fatigue factor (G*sin δ) at 5000 kPa, which was carried out using a pair of 8 mm parallel plates with a 1 mm gap at a control strain of 1%, an angular frequency of 10 rad/s, and a temperature range of 5~30 • C; (3) temperature response of viscoelastic behavior was tested using the above similar conditions at 6~30 • C and 30~62 • C, respectively; (4) Frequency response of viscoelastic behavior, following the above similar methods, was also tested in the frequency range of 0.628~188.1 rad/s at low temperature (6 • C), medium temperature (30 • C), and high temperature (62 • C), to study the rheological behaviors of bitumen samples under different climate environments.

Effect of Reaction Rejuvenation on Molecular Structure of aSBSmB
FTIR spectra of SBSmB before and after aging and rejuvenation are displayed in Figure 2. In addition, the attribution of its main characteristic peaks is shown in Table 2. As seen in curves a and b, it is easy to find that, after aging, the appearance of the peaks at 1696 cm −1 , 1014 cm −1 and 965 cm −1 are attributed to the stretching vibration of C=O, S=O and C=C, respectively. In addition, the appearance of the characteristic peak at 699 cm −1 was attributed to the bending vibration of C-H on the monosubstituted benzene ring. After aging, the characteristic absorption peaks at 699 cm −1 and 965 cm −1 belonging to the mono substituted benzene ring on the polystyrene segment still existed, indicating that as the thermo-oxidative aging time prolongs, the high-temperature conditions would not damage the benzene ring structure in the polystyrene segment of SBS. Meanwhile, the intensity of characteristic peaks attributed to the respiratory vibration of the benzene ring skeleton and the deformation vibration of C-H at 1260 cm −1 on the structure of Olefins decreased to a certain extent, indicating that aging promoted the oxidative degradation of SBS in SBSmB. When 3 wt% PU was added to aSBSmB, marked changes appeared in their corresponding spectrum. The characteristic peak at 2275 cm −1 is generated by the asymmetric stretching vibration of -NCO, and its intensity is obviously smaller, while the intensity of C=O is slightly enhanced. It indicates that when the rejuvenator amount of PU is 3 wt%, PU can completely react with the active oxygen-containing groups (such as -OH and -COOH) in aSBSmB, especially the oxidative degradation products of SBS. As seen in curves c and d, compared to 3PU/aSBSmB, the characteristic peak positions have no changes with the addition of AO, except for the disappearance of the characteristic peak attributed to the -NCO at 2275 cm −1 . This shows that the chemical composition of AO is similar to that of bitumen, having a few groups that can react with PU in mixtures, which basically indicates that AO acts as a physical softening effect on the rejuvenation of aSBSmB. basically indicates that AO acts as a physical softening effect on the rejuvenation of aS-BSmB.

Figure 2.
Effect of different rejuvenators on the molecular structure of aSBSmB.  Figure 3 shows the influence of reaction rejuvenation on the viscosity of aSBSmB. It can be seen that the viscosity of SBSmB increases after aging, which indicates that the workability of SBSmB worsens after aging. The viscosity of aSBSmB at 170 °C increased significantly from 675 mPa·s to 2140 mPa·s, and even reached 1450 mPa·s at 180 °C after adding 3 wt% PU, which indicated that PU would adversely affect the workability of aS-BSmB after rejuvenation. This is because PU reacts violently with the chemically active components in aSBSmB, forming a structural reinforcement with weakened high-temperature sensitivity. When 10 wt% AO was added to 3PU/aSBSmB, the viscosity of 3PU/aS-BSmB decreased from 2140 mPa·s to 1540 mPa·s and from 1450 mPa·s to 791 mPa·s at 170 °C and 180 °C , respectively. The results are due to the fact that 10 wt% AO as rejuvenator can compensate for the reduction of light components by aging volatilization or reaction in aSBSmB. In addition, the dilution and dissolution of AO reduces the viscosity and hardness of 3PU/aSBSmB. From this result, it is believed that the combined use of PU and AO contributes to better workability of the rejuvenated binder for mixing and construction. It is worthwhile noting that at both 170 °C and 180 °C, the viscosity of the rejuvenated binder is still higher than that of the fresh binder, but this still satisfies the mixing and compaction requirements of the asphalt mixture.   Figure 3 shows the influence of reaction rejuvenation on the viscosity of aSBSmB. It can be seen that the viscosity of SBSmB increases after aging, which indicates that the workability of SBSmB worsens after aging. The viscosity of aSBSmB at 170 • C increased significantly from 675 mPa·s to 2140 mPa·s, and even reached 1450 mPa·s at 180 • C after adding 3 wt% PU, which indicated that PU would adversely affect the workability of aSBSmB after rejuvenation. This is because PU reacts violently with the chemically active components in aSBSmB, forming a structural reinforcement with weakened hightemperature sensitivity. When 10 wt% AO was added to 3PU/aSBSmB, the viscosity of 3PU/aSBSmB decreased from 2140 mPa·s to 1540 mPa·s and from 1450 mPa·s to 791 mPa·s at 170 • C and 180 • C, respectively. The results are due to the fact that 10 wt% AO as rejuvenator can compensate for the reduction of light components by aging volatilization or reaction in aSBSmB. In addition, the dilution and dissolution of AO reduces the viscosity and hardness of 3PU/aSBSmB. From this result, it is believed that the combined use of PU and AO contributes to better workability of the rejuvenated binder for mixing and construction. It is worthwhile noting that at both 170 • C and 180 • C, the viscosity of the rejuvenated binder is still higher than that of the fresh binder, but this still satisfies the mixing and compaction requirements of the asphalt mixture.   Figure 4 shows the viscosity-temperature regression curves of virgin, aged and rejuvenated SBSmB, of which the linear fitting equations, regression coefficients and correlation coefficients are shown in Table 3. The correlation coefficients R 2 of the viscosity-temperature curves after linear fitting are not less than 0.95, indicating that the linear fitting curves can truly reflect the relationship between viscosity and temperature of virgin, aged and rejuvenated SBS modified bitumen. When SBSmB is aged, the regression coefficient (the value of m) increases from 1.293 to 1.446, indicating that the viscosity-temperature sensitivity of SBSmB enhance significantly after aging. This is mainly due to the loss of light components in the aSBSmB, resulting in a larger molecular weight of the bitumen matrix and a harder texture of the SBS modified asphalt binder. With the addition of 3 wt% of PU as rejuvenator, the value of m of the reaction-rejuvenated SBS modified asphalt binder decreased to 0.951, indicating that the addition of PU will reduce the viscositytemperature sensitivity. This is because PU reacts violently with the chemically active components in aSBSmB to make the molecules rotate relatively and does not harden the SBSmB after structural reconstruction, so as to reduce the viscosity-temperature sensitivity. After 10 wt% AO was added to the above 3PU/aSBSmB, it was found that the value of m is restored to 1.459, indicating that the addition of AO can enhance the viscosity-temperature sensitivity of 3PU/aSBSmB for better workability.  Figure 4 shows the viscosity-temperature regression curves of virgin, aged and rejuvenated SBSmB, of which the linear fitting equations, regression coefficients and correlation coefficients are shown in Table 3. The correlation coefficients R 2 of the viscosity-temperature curves after linear fitting are not less than 0.95, indicating that the linear fitting curves can truly reflect the relationship between viscosity and temperature of virgin, aged and rejuvenated SBS modified bitumen. When SBSmB is aged, the regression coefficient (the value of m) increases from 1.293 to 1.446, indicating that the viscosity-temperature sensitivity of SBSmB enhance significantly after aging. This is mainly due to the loss of light components in the aSBSmB, resulting in a larger molecular weight of the bitumen matrix and a harder texture of the SBS modified asphalt binder. With the addition of 3 wt% of PU as rejuvenator, the value of m of the reaction-rejuvenated SBS modified asphalt binder decreased to 0.951, indicating that the addition of PU will reduce the viscosity-temperature sensitivity. This is because PU reacts violently with the chemically active components in aSBSmB to make the molecules rotate relatively and does not harden the SBSmB after structural reconstruction, so as to reduce the viscosity-temperature sensitivity. After 10 wt% AO was added to the above 3PU/aSBSmB, it was found that the value of m is restored to 1.459, indicating that the addition of AO can enhance the viscosity-temperature sensitivity of 3PU/aSBSmB for better workability.

Variation of Integrity Parameter (C) with Cumulative Fatigue Damage Parameter (D)
The initial integrity (C) without damage is determined as a value of 1, and 0 represents the complete damage of the binder. For a specific D value, the lower the C value, the higher the damage degree of bitumen, and the worse the fatigue damage resistance of bitumen. Figure 5 shows the relationship between the integrity parameter (C) and cumulative fatigue damage parameter (D) of the virgin, aged, and rejuvenated SBSmB. After aging, the integrity curve of SBSmB becomes steeper, which indicates that the loss rate is significantly increased, and the fatigue resistance is worse than that of virgin SBSmB. When 3 wt% PU was added, the fatigue resistance performance of aSBSmB was visually reduced. This may be due to the negative influence of PU on the colloidal structure of aged SBSmB. By contrast, the combined use of PU and AO promotes not only the rejuvenation of network structure, but also the restoration of bitumen fractions in aged SBSmB, leading to the better resistance of 3PU/10AO/aSBSmB to fatigue.

Variation of Integrity Parameter (C) with Cumulative Fatigue Damage Parameter (D)
The initial integrity (C) without damage is determined as a value of 1, and 0 represents the complete damage of the binder. For a specific D value, the lower the C value, the higher the damage degree of bitumen, and the worse the fatigue damage resistance of bitumen. Figure 5 shows the relationship between the integrity parameter (C) and cumulative fatigue damage parameter (D) of the virgin, aged, and rejuvenated SBSmB. After aging, the integrity curve of SBSmB becomes steeper, which indicates that the loss rate is significantly increased, and the fatigue resistance is worse than that of virgin SBSmB. When 3 wt% PU was added, the fatigue resistance performance of aSBSmB was visually reduced. This may be due to the negative influence of PU on the colloidal structure of aged SBSmB. By contrast, the combined use of PU and AO promotes not only the rejuvenation of network structure, but also the restoration of bitumen fractions in aged SBSmB, leading to the better resistance of 3PU/10AO/aSBSmB to fatigue. The numbers of cycles at fatigue failure of SBSmB before and after aging and after rejuvenation is shown in Figure 6 and Table 4. It is clear that the curve slope of aSBSmB is bigger than that of the fresh binder, indicating that the fatigue life of aSBSmB is by contrast  The numbers of cycles at fatigue failure of SBSmB before and after aging and after rejuvenation is shown in Figure 6 and Table 4. It is clear that the curve slope of aSBSmB is bigger than that of the fresh binder, indicating that the fatigue life of aSBSmB is by contrast more sensitive to load. As PU precursor plays an important role in the rejuvenation, its rejuvenated binder shows a higher fatigue life compared to aged one at a smaller strain, such as below 1%, because of its reaction-enhancing effects from the chemical rejuvenation of degradation products. In addition, N f of 3PU/10AO/aSBSmB presents a higher value than that of 3PU/aSBSmB at higher strain of over 1%, which further demonstrates that AO can help significantly improve the fatigue resistance of PU rejuvenated binder at high strains. Overall, the combined use of PU and AO can positively contribute to enhancing the fatigue properties of aged binder, particularly at higher stains.

Number of Cycles to Fatigue Failure ( f )
The numbers of cycles at fatigue failure of SBSmB before and after aging and after rejuvenation is shown in Figure 6 and Table 4. It is clear that the curve slope of aSBSmB is bigger than that of the fresh binder, indicating that the fatigue life of aSBSmB is by contrast more sensitive to load. As PU precursor plays an important role in the rejuvenation, its rejuvenated binder shows a higher fatigue life compared to aged one at a smaller strain, such as below 1%, because of its reaction-enhancing effects from the chemical rejuvenation of degradation products. In addition, of 3PU/10AO/aSBSmB presents a higher value than that of 3PU/aSBSmB at higher strain of over 1%, which further demonstrates that AO can help significantly improve the fatigue resistance of PU rejuvenated binder at high strains. Overall, the combined use of PU and AO can positively contribute to enhancing the fatigue properties of aged binder, particularly at higher stains.   Figures 7 and 8, respectively, reflect the influence of reaction rejuvenation on antirutting deformation and the anti-fatigue characteristics of aSBSmB. It can be seen that the 76 • C rutting factor and fatigue failure temperature of SBSmB after aging both increase significantly, from 1.83 kPa to 6.09 kPa and from 17.8 • C to 24.0 • C, respectively, which indicates that the deformation resistance of SBSmB can be improved after aging, but its fatigue property is prone to failure at higher temperatures. With the addition of 3 wt% PU, the rutting factor of aSBSmB at 76 • C increased significantly from 6.09 kPa to 14.06 kPa, with an increase of 130.9%, and its fatigue failure temperature increased to 27.0 • C, indicating that PU can significantly improve the deformation resistance of aSBSmB, but it will also reduce its fatigue resistance to some extent. Therefore, when 10 wt% AO is added to 3PU/aSBSmB, the rutting factor of rejuvenated SBSmB at 76 • C can still be kept at 5.17 kPa, and its fatigue failure temperature (16.4 • C) is lower than that of the virgin SBSmB (17.8 • C), which indicates that the synergistic rejuvenation effect of PU and AO can not only ensure the hightemperature stability of rejuvenated SBSmB, but can also promote its ability to resist fatigue damage. This is because the chemical reaction between PU and SBS oxidation degradation products dominates the high-temperature characteristics of rejuvenated SBSmB, while AO, as a softening agent of hard components in aged bitumen, supplements the light components, which positively affects the fatigue performance of rejuvenated SBSmB.

Evaluation of Anti-Deformation and Fatigue Performance of Reaction Rejuvenation SBSmB
fatigue property is prone to failure at higher temperatures. With the addition of 3 wt% PU, the rutting factor of aSBSmB at 76 °C increased significantly from 6.09 kPa to 14.06 kPa, with an increase of 130.9%, and its fatigue failure temperature increased to 27.0 °C , indicating that PU can significantly improve the deformation resistance of aSBSmB, but it will also reduce its fatigue resistance to some extent. Therefore, when 10 wt% AO is added to 3PU/aSBSmB, the rutting factor of rejuvenated SBSmB at 76 °C can still be kept at 5.17 kPa, and its fatigue failure temperature (16.4 °C ) is lower than that of the virgin SBSmB (17.8 °C ), which indicates that the synergistic rejuvenation effect of PU and AO can not only ensure the high-temperature stability of rejuvenated SBSmB, but can also promote its ability to resist fatigue damage. This is because the chemical reaction between PU and SBS oxidation degradation products dominates the high-temperature characteristics of rejuvenated SBSmB, while AO, as a softening agent of hard components in aged bitumen, supplements the light components, which positively affects the fatigue performance of rejuvenated SBSmB.   Figure 9 shows the temperature response of the viscoelastic behavior of SBSmB. It can be seen from Figure 9a that after aging, the complex modulus of SBSmB obviously increases within the design temperature range. When 3 wt% PU was added to aSBSmB, its complex modulus increased slightly, but after adding 10 wt% AO, the complex modulus of rejuvenated SBSmB was slightly higher than that of virgin SBSmB. These results showed that the synergistic reaction and rejuvenation of PU and AO can make the deformation resistance of aged SBSmB slightly higher than that of the virgin SBSmB. The reason for this result is consistent with the analysis of the performance results obtained in Sec-  Figure 9 shows the temperature response of the viscoelastic behavior of SBSmB. It can be seen from Figure 9a that after aging, the complex modulus of SBSmB obviously increases within the design temperature range. When 3 wt% PU was added to aSBSmB, its complex modulus increased slightly, but after adding 10 wt% AO, the complex modulus of rejuve-nated SBSmB was slightly higher than that of virgin SBSmB. These results showed that the synergistic reaction and rejuvenation of PU and AO can make the deformation resistance of aged SBSmB slightly higher than that of the virgin SBSmB. The reason for this result is consistent with the analysis of the performance results obtained in Sections 3.3 and 3.4 above. In addition, from Figure 9b, the elastic modulus G or viscous modulus G" of SBSmB before and after aging and rejuvenation is consistent with the change law of its corresponding complex modulus, except that its viscoelastic transition temperature (that is, the temperature corresponding to the intersection of G -T and G"-T curve) is different. It showed that the viscoelastic transition temperature of SBSmB increases from 11.8 • C to 19.9 • C after aging. Further, 3 wt% PU promoted the viscoelastic transition temperature of aSBSmB to continue to increase to 25.2 • C. Then, when 10 wt% AO was added to 3PU/aSBSmB, this value decreased to 12.4 • C, and basically returned to the virgin SBSmB level. These results indicate that the interaction between PU and aSBSmB will lead to the elastic behavior of PU rejuvenated SBSmB, and the elastic behavior of rejuvenated SBSmB will gradually develop to viscous behavior after the softening action of appropriate amount of AO, showing the viscoelastic behavior characteristics close to the virgin SBSmB. The main reason for this result is the chemical interaction between PU and oxidation degradation products of SBS after aging, which organically reconstructs the molecular structure of the modifier and forms the crosslinked structure with relatively difficult molecular movement. Then, through the permeation plasticization of AO, the intermolecular force of aging asphalt is reduced, and the rejuvenated SBSmB with stable physical and chemical structure is achieved.  Figure 10 shows the frequency response of viscoelastic behavior of SBSmB at different temperatures. It can be seen that the addition of 3 wt% PU will increase the complex modulus of aSBSmB in the set frequency range (0.628~88.1 rad/s) regardless of the ambient temperature. However, after adding 10 wt% AO continuously, the frequency response of the complex modulus of rejuvenated SBSmB at different temperatures is different, specifically, its viscoelastic behavior is very close to the level of the virgin SBSmB at low temperature; when the temperature transits from low temperature to medium temperature, its viscoelastic behavior, which is characterized by elasticity, gradually approaches the level of the virgin SBSmB with the increase of frequency. At high temperature, its elastic resistance behavior is dominant, which is higher than that of the virgin SBSmB. These results show that the frequency response of SBSmB rejuvenated with an appropriate amount of PU and AO is similar to that of the virgin SBSmB in a low-temperature environment, but it mainly shows a stronger frequency response than that of the virgin SBSmB in medium-and high-temperature environments. This is because, at low temperature, the movement of small molecule AO provides internal plasticization for the stable structure rebuilt by PU and the aged bitumen molecules, which makes the rejuvenated SBSmB obtain the viscoelastic characteristics equivalent to the virgin SBSmB. At medium and high  Figure 10 shows the frequency response of viscoelastic behavior of SBSmB at different temperatures. It can be seen that the addition of 3 wt% PU will increase the complex modulus of aSBSmB in the set frequency range (0.628~88.1 rad/s) regardless of the ambient temperature. However, after adding 10 wt% AO continuously, the frequency response of the complex modulus of rejuvenated SBSmB at different temperatures is different, specifically, its viscoelastic behavior is very close to the level of the virgin SBSmB at low temperature; when the temperature transits from low temperature to medium temperature, its viscoelastic behavior, which is characterized by elasticity, gradually approaches the level of the virgin SBSmB with the increase of frequency. At high temperature, its elastic resistance behavior is dominant, which is higher than that of the virgin SBSmB. These results show that the frequency response of SBSmB rejuvenated with an appropriate amount of PU and AO is similar to that of the virgin SBSmB in a low-temperature environment, but it mainly shows a stronger frequency response than that of the virgin SBSmB in mediumand high-temperature environments. This is because, at low temperature, the movement of small molecule AO provides internal plasticization for the stable structure rebuilt by PU and the aged bitumen molecules, which makes the rejuvenated SBSmB obtain the viscoelastic characteristics equivalent to the virgin SBSmB. At medium and high temperature, although the movement of AO molecules intensifies, the rejuvenated crosslinked structure of SBS degradation products rebuilt by PU shows stable high-temperature characteristics. To further clarify the above viewpoint, the frequency response of viscoelastic transition of reaction-rejuvenated SBSmB is shown in Figure 11. It can be seen that with the increasing frequency, the virgin SBSmB has a tendency to change from viscous behavior to elastic behavior at about 2.5 rad/s at low temperature, and other binders present a tendency of elastic behavior in the whole frequency and temperature range. In addition, at low temperature, the elastic modulus and viscous modulus of the rejuvenated SBSmB are close to those of the virgin SBSmB, while at medium and high temperature, the elastic modulus and viscous modulus of the rejuvenated SBSmB are both higher than that of virgin SBSmB. It indicates that compared to virgin SBSmB, the rejuvenated SBSmB basically has the similar viscoelastic behavior at low temperature, and it has better ability to resist elastic deformation at medium and high temperature. The reason for this result is consistent with the above analysis.

Conclusions
(1) This study proposed a new physicochemical rejuvenation method based on the novel idea of rebuilding the molecular structure of aged SBS. PU prepolymer was used as a reactive substance to react with active oxygen-containing groups from the degradation products of SBS, and AO was used as a common rejuvenator to supplement the lost light fractions of asphalt molecules in aged SBSmB. With respect to the structure and performance characterizations, a series of tests, including infrared spectra, viscosity, and dynamic shear rheology, were carried out for the rejuvenation analysis of aged SBSmB. Based on this, the main conclusions can be drawn: FTIR results indicated that PU can react with oxidative degradation products of SBS, such as -OH and -COOH, for structural reconstruction, while AO can soften the aged virgin bitumen through the reduction of heavy fractions. (2) RV results suggested that the increased viscosity of aged SBSmB after adding PU can be effectively decreased to a better workability with a certain incorporation of PU.
(3) LAS results demonstrated that the combined use of PU and AO can reach a better resistance of aged SBSmB to fatigue by contrast to single use of PU, because of chemical rejuvenation of the network structure of aged SBS and the physical softening rejuvenation of aged bitumen components. (4) Combined results of rutting and fatigue factors stated that the chemical reaction between PU and SBS degradation products dominates the high-temperature stability of rejuvenated SBSmB, while AO supplements the light components in aged bitumen and improves the fatigue performance of rejuvenated SBSmB.